A new attempt to adopt a machine for SHS lining ceramics inside pipes Reza Mahmoodiana,c,d*, R. G. Rahbarib , M. Hamdia,c ,Mahdi Sparhama,c
* Department of Engineering Design and Manufacture, University of Malaya, 50603 Kuala Lumpur, Malaysia
Email: email@example.com, firstname.lastname@example.org
Contact Details: Phone: 0060(3) 79675200, Fax: 0060(3) 79675330
Department of Engineering Design and Manufacture, University of Malaya, 50603 Kuala Lumpur,
Restorative Dentistry Department, Dentistry Faculty, University of Toronto, Toronto, ON M5G1G6,
Centre of Advanced Manufacturing and Materials Processing (AMMP), University of Malaya, 50603
Kuala Lumpur, Malaysia, email@example.com
Department of Research and Development, Azarin Kar Ind. Co., Industrial Zone 1, 7635168361 Kerman,
A new attempt to adopt a machine for SHS lining ceramics inside pipes
In order to conduct centrifugal thermite research experiments in the laboratory, a special apparatus is required. A self-propagating high temperature synthesis machine with acceleration up to 350g was fabricated to accomplish experiments in laboratory settings. Then, thermite reaction of Ferro oxide III and Aluminium inside a pipe was performed to produce Alumina ceramic in the innermost layer and Ferro layer. Combustion synthesis is characterized by extreme heating rate, high temperature, and short reaction time. Centrifugal force facilitated the phase separation of multi-component products during the process. Preliminary tests were conducted prior to fabrication to realize reaction conditions.
Keywords: Ceramic-lined pipes; Centrifugal; Self-propagating high-temperature synthesis; SHS; Combustion synthesis; Thermite
The self-propagating high-temperature synthesis (SHS) technique results in the in situ creation of composites from reactant substances through exothermic chemical reaction. The heat generated by the exothermic reaction to ignite and sustain a propagating combustion wave through the reactants creates the anticipated product (Fan et al. 2006; Graeve and Munir 2002; Ivleva et al. 2011; Kanakala et al. 2011; Odawara 1990; Odawara 2010; Pei et al. 2009; Salonitis et al. 2010; Wang and Yang 2007). SHS processes are characterized by high-temperatures; these characteristics make SHS an economical method for the industries compared to conventional ceramic processing. SHS is a feasible technique for preparing advanced ceramics, catalysts, and nanomaterials (Munoz et al. 1997; Patil et al. 1997; Sun et al. 2008). Ceramic-lined composite pipe is a high-performance, heat-resistant, anti-corrosion and wear-resistant pipe that can be produced through the centrifugal SHS process which is spontaneous reaction propagation and rapid synthesis under the effect of centrifugal force. The reaction occurs in the inner pipe surface after melting the Aluminum in the first stage. The self-sustained exothermic chemical reaction propagates through a premixed powder in the form of a high temperature reaction wave with fast heating rates and short reaction times. Then it would be followed by phase separation and solidification of Al2O3 and Fe products. The product of centrifugal SHS reaction between Fe2O3 and Al is a metal-ceramic composite of Al2O3-Fe (Odawara et al. 1989; Rogachev and Baras 2007; Xu et al. 2010).
The adiabatic combustion temperature of the centrifugal SHS reaction can reach up to 2400ºC which is higher than the melting points of Al and Fe2O3 (Chatterjee et al. 2008; Patil et al. 1997; Sun et al. 2008). The advantage of this process is that once ignited, no further externally applied energy is necessary.
Processing time is reduced, and the products are normally of high purity (Chatterjee et al. 2008; Merzhanov 1990; Yu et al. 2010).
The simple, rapid, and economical centrifugal SHS process was used to produce various types of metal-ceramic composite pipes. Ceramic-lined pipes are applied in several fields such as petrochemical,
Developing a test rig was necessary to conduct more research on centrifugal SHS products. In the current research work, a test rig was designed and fabricated to facilitate the study after performing a few
preliminary experiments. The apparatus is as simple as possible to maintain the SHS process concept feasible and so it can be adopted in a wide range of exothermic ceramic lining techniques in laboratories. This apparatus facilitates research work in the field of centrifugal SHS process in industrial and educational fields.
2. Test Rig Fabrication
A centrifugal machine was designed to facilitate the SHS experiment utilized for laboratory-scale production of ceramic-lined steel pipes. Rotation speed, simplicity of use, ergonomic and safety factors, stability, and low vibration aspects were considered in machine development. The technical requirements for high-temperature and high-speed reactions in the small chamber were determined during preliminary tests.
2.1. Apparatus Design
Anthropometry information collected from 32 students in the 2007-2008 session at University of Malaya was adopted for the test rig design. It is expected to cover 95% of the population of potential users in terms of hand grip area and height (Schlick 2009). A cross-sectional view of the designed centrifugal machine is shown in Figure 1. The machine would have to undergo high centrifugal acceleration and rapid temperature rise during experiment. The steel pipe must be fixed inside the reaction chamber as shown in Figure 1.
Figure 1: A cross-sectional view of the designed test rig
inverter can control the reaction chamber’s rotational speed in order to provide the required centrifugal acceleration which can reach from a=2g up to a=380g.
3. Experimental Procedure
The fabricated centrifugal machine was used for the production of ceramic coating in metallic pipes. Aluminum (< 75μm, 99% purity, Sigma Aldrich) and Fe2O3 (< 5μm, 97% purity, Sigma Aldrich) powders were dried for eight hours and mixed for 5 hours at a speed of 35rpm. The green powder stoichiometry mixture was kept based on equation (1):
2 3 2 3
Fe O +2Al→ Al O +2Fe + 836 kJ
A carbon steel pipe with a length of 110mm, inner and outer diameters of 69mm and 75mm, respectively, was used. The pipe was fixed inside the reaction chamber, while a refractory cap was attached to the pipe head. The pipe was charged with the green powder mixture while rotating at low speed. During the experiment, an embedded speedometer monitored the rotational speed of the pipe in the centrifugal SHS machine. Ignition of the charged powder mixture in the pipe was initiated by Oxyacetylene gas. The rotational speed was kept constant at centrifugal acceleration of a = 250g during reaction to ensure reaction uniformity and completion inside the pipe. The overall experimental setup scheme before and after reaction is shown in
Figure 2: Schematic diagram illustrating steel pipe charged with a green mixture before reaction (left) and after reaction (right) while subject to centrifugal force
Normally, the SHS reaction is rather violent (Li et al. 2005), a sign that the reaction is beginning inside the pipe. In order to reduce reaction violence, Al2O3 was added to the mixture as inert diluent (Orru et al. 1996). The exothermic reaction between Fe2O3 and Al inside the pipe produced high temperature Al2O3 solid ceramic and molten Fe. Phase formation of products was followed by phase separation under the centrifugal force at high rotational speed (Orru et al. 1996; Yukhvid 1992). The pipe was kept rotating at the same rotational speed since the start of reaction until product solidification was complete. The cooled ceramic–lined composite pipe was taken out for characterization. Micro-hardness of the ceramic layer was measured at different points on the ceramic layer surface.
4. Results and Discussion
during the reaction as well. In the preliminary experiments, due to high the temperature gradient, pipe deformations were observed due to the softening of pipe walls. There are six holes considered in the
reaction chamber wall (Figure 1) in order to ease the airflow and reduce pipe deformation by disseminating the heat generated during reaction.
Figure 3: Photographic view of a typical product of centrifugal SHS reaction
A Bruker D8 Advance with a monochromatic Cu Kα source was employed for X-ray composition analysis of the ceramic layer surface. The X-ray diffraction pattern of the obtained products (Figure 4) elicits the formation of Al2O3 (Corundum), Fe and AlFe3. In Figure 4, the most intensive peak of Al2O3 was detected at 2θ=37.69°.
Figure 4: X-ray diffraction pattern of the centrifugal SHS products on inner surface
Figure 5: SEM micrograph of the boundary between ceramic and metallic layers
The hardness varies from point to point due to heterogeneity in phase-structure distribution in the inner surface of the ceramic layer. Hardness variation is directly related to the concentration of pores. The maximum hardness value recorded was 2365HV. Pipe curvature influences the compressive and tensile stresses generated in the layers (Odawara 1990). However, the bonding between layers and their
mechanical characteristics present a successful process performed by the developed test rig.
The fabricated test rig seems feasible to be used in the laboratory in order to prepare ceramic-coated pipes using the centrifugal SHS method. Preliminary tests prior to fabrication improved the quality of the developed centrifugal SHS test rig. The apparatus can produce a wide range of SHS activating powders under different centrifugal accelerations and parameters. Phase formation was verified by XRD and SEM tests. Mechanically interlocking bonding was observed in different phases, which helped improve the bonding strength.
This project has been done under High Impact Grant (HIR-MOHE-D0001-16001) University of Malaya. Special thanks to Mr. Ali Mahmoodian the CEO of Azarin Kar Ind. Co. to consult and facilitate SHS-centrifugal machine design and fabrication.
Andreev, D., V. Sanin, et al.,(2011) Cermet-lined tubes from industrial wastes by centrifugal SHS,
International Journal of Self-Propagating High-Temperature Synthesis 20(1), pp. 27-32. Chatterjee, S., S. Shariff, et al.,(2008) Development of nano-structured Al2O3-TiB2-TiN coatings by
combined SHS and laser surface alloying, The International Journal of Advanced Manufacturing Technology 38(9), pp. 938-943.
Fan, R.-H., H.-L. Lü, et al.,(2006) Kinetics of thermite reaction in Al-Fe2O3 system, Thermochimica Acta
440(2), pp. 129-131.
Graeve, O. A. and Z. A. Munir,(2002) The effect of an electric field on the microstructural development during combustion synthesis of TiNi–TiC composites, Journal of Alloys and Compounds 340(1–2), pp. 79-87.
Kanakala, R., R. Escudero, et al.,(2011) Mechanisms of Combustion Synthesis and Magnetic Response of High-Surface-Area Hexaboride Compounds, ACS Applied Materials & Interfaces 3(4), pp. 1093-1100.
Lai, W., Z. A. Munir, et al.,(1997) Centrifugally-assisted combustion synthesis of functionally-graded materials, Scripta Materialia 36(3), pp. 331-334.
Li, P., E. G. Kandalova, et al.,(2005) In situ synthesis of Al-TiC in aluminum melt, Materials Letters
59(19-20), pp. 2545-2548.
Merzhanov, A. G.,(1990) Self-propagating high-temperature synthesis: twenty years of search and findings. California: VCH.
Munir, Z. A., W. N. Lai, et al.,(2000). Centrifugal synthesis and processing of functionally graded materials, USA Patent. USA, The Regents of the University of California, Oakland, Calif. Munoz, J. D., A. Arizmendi, et al.,(1997) High temperature activation energy for plastic deformation of
titanium carbide single crystals as a function of the C : Ti atom ratio, JOURNAL OF MATERIALS SCIENCE 32(12), pp. 3189-3193.
Odawara, O.,(1990) Long Ceramic-Lined Pipes Produced by a Centrifugal-Thermit Process, Journal of the American Ceramic Society 73(3), pp. 629-633.
Odawara, O.,(2010) Mass-Forced SHS Technology of Ceramic Materials, Advances in Science and Technology 63, pp. 302-311.
Odawara, O., Y. Taneoka, et al.,(1989) Combustion Synthesis of the Titanium-Aluminum-Boron System,
Journal of the American Ceramic Society 72(6), pp. 1047-1049.
Orru, R., B. Simoncini, et al.,(1996) Computer-aided manufacturing of centrifugal SHS coatings,
Computers & Chemical Engineering 20(Supplement 2), pp. S1185-S1190.
Patil, K. C., S. T. Aruna, et al.,(1997) Combustion synthesis, Current Opinion in Solid State and Materials Science 2(2), pp. 158-165.
Pei, J., J.-T. Li, et al.,(2009) Fabrication of bulk Al2O3 by combustion synthesis melt-casting under ultra-high gravity, Journal of Alloys and Compounds 476(1-2), pp. 854-858.
Rogachev and Baras,(2007) Models of SHS: An Overview, International Journal of Self-Propagating High-Temperature Synthesis 16(3), pp. 141-153.
Salonitis, K., J. Pandremenos, et al.,(2010) Multifunctional materials: engineering applications and processing challenges, The International Journal of Advanced Manufacturing Technology 49(5), pp. 803-826.
Schlick, C. M.,(2009) Industrial Engineering and Ergonomics: Visions, Concepts, Methods and Tools Festschrift in Honor of Professor Holger Luczak. Aachen, Germany: Springer Publishing Company, Incorporated.
Sun, L., A. Sneller, et al.,(2008) Fabrication of alumina/zirconia functionally graded material: From optimization of processing parameters to phenomenological constitutive models, Materials Science and Engineering: A 488(1-2), pp. 31-38.
Wang, Y.-F. and Z.-G. Yang,(2007) Finite element analysis of residual thermal stress in ceramic-lined composite pipe prepared by centrifugal-SHS, Materials Science and Engineering: A 460-461, pp. 130-134.
Xu, B., L. Zhang, et al.,(2010) Investigation on Al2O3/YSZ eutectic ceramics lining in the pipes prepared by combustion synthesis, Advanced Materials Research 105-106(1), pp. 12-15.
Yu, Z., S. Shugang, et al.,(2010) Study on Microstructure and Properties of Ceramic-lined Steel Pipes Prepared by Self-propagating High-temperature Centrifugal Process, Hot Working Technology. Yukhvid, V. I.,(1992) Modifications of SHS processes, Pure and Applied Chemistry 64(7), pp. 977-988. Zhou, Q., L. Xue, et al.,(2010) Microstructure of ceramic-lined composite steel pipe prepared by
SHS-centrifugal process, Tezhong Zhuzao Ji Youse Hejin/Special Casting and Nonferrous Alloys 30(7), pp. 671-673.
Zhou, Y., C.-J. Li, et al.,(2010) Effect of self-propagating high-temperature combustion synthesis on the deposition of NiTi coating by cold spraying using mechanical alloying Ni/Ti powder, Intermetallics